LMucko/crystallography-open-database huggingface dataset:
Lithium ion insertion and extraction reactions with Hollandite-type manganese dioxide free from any stabilizing cations in its tunnel cavity
Kijima, N.; Takahashi, Y.; Akimoto, J.; Awaka, J.; Journal of Solid State Chemistry 178 (2005) 2741–2750; doi:10.1016/j.jssc.2005.06.023

data_1514025
_publ_section_title
;
 Lithium ion insertion and extraction reactions with Hollandite-type
 manganese dioxide free from any stabilizing cations in its tunnel cavity
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              2741
_journal_page_last               2750
_journal_paper_doi               10.1016/j.jssc.2005.06.023
_journal_volume                  178
_journal_year                    2005
_chemical_formula_structural     '(Li2 O)0.12 (Mn O2)'
_chemical_formula_sum            'Li0.24 Mn O2.12'
_chemical_name_systematic
;
(dilithium Oxide) (manganese(IV) Oxide) (0.12/1)
;
_space_group_IT_number           87
_symmetry_Int_Tables_number      87
_symmetry_space_group_name_Hall  '-I 4'
_symmetry_space_group_name_H-M   'I 4/m'
_audit_creation_date             2006/10/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   9.993(11)
_cell_length_b                   9.993(11)
_cell_length_c                   2.853(3)
_cell_volume                     284.9(5)
_refine_ls_R_factor_all          0.0131
_cod_data_source_file            'data_LiMnO2melanie153165.cif'
_cod_data_source_block           LiMnO2melanie153165.cif
_cod_original_cell_volume        284.9
_cod_original_formula_sum        'Li0.24 Mn1 O2.12'
_cod_database_code               1514025
Li content dependence of thermodynamic stability abd the crystal structure of Lix Mn1-y My O2 (M = Mn, Al, Cu) as a cathode active material for Li secondary battery
Idemoto, Y.; Konno, Y.; Ui, K.; Koura, N.; Electrochemistry (Tokyo) 73 (2005) 823–829; doi:

data_1514026
_publ_section_title
;
 Li content dependence of thermodynamic stability abd the crystal
 structure of Lix Mn1-y My O2 (M = Mn, Al, Cu) as a cathode active
 material for Li secondary battery
;
_journal_coden_ASTM              EECTFA
_journal_issue                   9
_journal_name_full               'Electrochemistry (Tokyo)'
_journal_page_first              823
_journal_page_last               829
_journal_volume                  73
_journal_year                    2005
_chemical_formula_structural     'Li0.4 Mn O2'
_chemical_formula_sum            'Li0.4 Mn O2'
_chemical_name_systematic
;
Lithium Manganese Oxide (0.4/1/2) - I
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_audit_creation_date             2007/04/01
_audit_update_record             2013/02/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            16
_cell_length_a                   8.220(3)
_cell_length_b                   8.220(3)
_cell_length_c                   8.220(3)
_cell_volume                     555.4(4)
_refine_ls_R_factor_all          0.0452
_cod_data_source_file            'data_LiMnO2melanie154416.cif'
_cod_data_source_block           LiMnO2melanie154416.cif
_cod_original_cell_volume        555.41
_cod_original_sg_symbol_H-M      'F d -3 m S'
_cod_original_formula_sum        'Li0.4 Mn1 O2'
_cod_database_code               1514026
Li content dependence of thermodynamic stability abd the crystal structure of Lix Mn1-y My O2 (M = Mn, Al, Cu) as a cathode active material for Li secondary battery
Idemoto, Y.; Konno, Y.; Ui, K.; Koura, N.; Electrochemistry (Tokyo) 73 (2005) 823–829; doi:

data_1514027
_publ_section_title
;
 Li content dependence of thermodynamic stability abd the crystal
 structure of Lix Mn1-y My O2 (M = Mn, Al, Cu) as a cathode active
 material for Li secondary battery
;
_journal_coden_ASTM              EECTFA
_journal_issue                   9
_journal_name_full               'Electrochemistry (Tokyo)'
_journal_page_first              823
_journal_page_last               829
_journal_volume                  73
_journal_year                    2005
_chemical_formula_structural     'Li0.7 Mn O2'
_chemical_formula_sum            'Li0.7 Mn O2'
_chemical_name_systematic
;
Lithium Manganese Oxide (0.7/1/2) - Ii
;
_space_group_IT_number           59
_symmetry_Int_Tables_number      59
_symmetry_space_group_name_Hall  '-P 2ab 2a'
_symmetry_space_group_name_H-M   'P m m n :2'
_audit_creation_date             2007/04/01
_audit_update_record             2013/02/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            2
_cell_length_a                   4.656(6)
_cell_length_b                   2.832(6)
_cell_length_c                   5.766(14)
_cell_volume                     76.0(3)
_refine_ls_R_factor_all          0.0452
_cod_data_source_file            'data_LiMnO2melanie154417.cif'
_cod_data_source_block           LiMnO2melanie154417.cif
_cod_original_cell_volume        76.02
_cod_original_sg_symbol_H-M      'P m m n Z'
_cod_original_formula_sum        'Li0.7 Mn1 O2'
_cod_database_code               1514027
Properties, crystal structure and performance of o-(Li Mn O2) as cathode material for Li secondary batteries
Idemoto, Y.; Mochizuki, T.; Ui, K.; Koura, N.; Journal of the Electrochemical Society 153 (2006) A418–A424; doi:10.1149/1.2142293

data_1514028
_publ_section_title
;
 Properties, crystal structure and performance of o-(Li Mn O2) as cathode
 material for Li secondary batteries
;
_journal_coden_ASTM              JESOAN
_journal_issue                   2
_journal_name_full               'Journal of the Electrochemical Society'
_journal_page_first              A418
_journal_page_last               A424
_journal_paper_doi               10.1149/1.2142293
_journal_volume                  153
_journal_year                    2006
_chemical_formula_structural     'Li (Mn O2)'
_chemical_formula_sum            'Li Mn O2'
_chemical_name_systematic        'Lithium Manganate(III) - O'
_space_group_IT_number           59
_symmetry_Int_Tables_number      59
_symmetry_space_group_name_Hall  '-P 2ab 2a'
_symmetry_space_group_name_H-M   'P m m n :2'
_audit_creation_date             2007/04/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            2
_cell_length_a                   4.5757(4)
_cell_length_b                   2.8058(2)
_cell_length_c                   5.7490(6)
_cell_volume                     73.809(11)
_refine_ls_R_factor_all          0.0482
_cod_data_source_file            'data_LiMnO2melanie154823.cif'
_cod_data_source_block           LiMnO2melanie154823.cif
_cod_original_cell_volume        73.81
_cod_original_sg_symbol_H-M      'P m m n Z'
_cod_original_formula_sum        'Li1 Mn1 O2'
_cod_database_code               1514028
Cation distribution, structure and magnetic properties of lithium manganese iron oxide spinel solid solutions
Wende, C.; Olimov, Kh.; Modrow, H.; Wagner, F. E.; Langbein, H.; Materials Research Bulletin 41 (2006) 1530–1542; doi:10.1016/j.materresbull.2006.01.016

data_1514029
_publ_section_title
;
 Cation distribution, structure and magnetic properties of lithium
 manganese iron oxide spinel solid solutions
;
_journal_coden_ASTM              MRBUAC
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              1530
_journal_page_last               1542
_journal_paper_doi               10.1016/j.materresbull.2006.01.016
_journal_volume                  41
_journal_year                    2006
_chemical_formula_structural     'Li Mn2 O4'
_chemical_formula_sum            'Li Mn2 O4'
_chemical_name_systematic
;
Lithium Manganese(III) Manganese(IV) Oxide
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2007/04/01
_audit_update_record             2010/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.24726(10)
_cell_length_b                   8.24726(10)
_cell_length_c                   8.24726(10)
_cell_volume                     560.956(12)
_refine_ls_R_factor_all          0.0411
_cod_data_source_file            'data_LiMn2O4melanie155282.cif'
_cod_data_source_block           LiMn2O4melanie155282.cif
_cod_original_cell_volume        560.96
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'Li1 Mn2 O4'
_cod_database_code               1514029
Li Mn2-x Tix O4 spinel-type compounds (x <= 1): structural, electrical and magnetic properties
Krins, N.; Hatert, F.; Traina, K.; Dusoulier, L.; Molenberg, I.; Fagnard, J. F.; Vanderbemden, P.; Rulmont, A.; Cloots, R.; Vertruyen, B.; Solid State Ionics 177 (2006) 1033–1040; doi:10.1016/j.ssi.2006.04.001

data_1514030
_publ_section_title
;
 Li Mn2-x Tix O4 spinel-type compounds (x <= 1): structural, electrical
 and magnetic properties
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              1033
_journal_page_last               1040
_journal_paper_doi               10.1016/j.ssi.2006.04.001
_journal_volume                  177
_journal_year                    2006
_chemical_formula_structural     'Li0.94 (Mn2.034 O4)'
_chemical_formula_sum            'Li0.94 Mn2.034 O4'
_chemical_name_systematic
;
Lithium Manganese Oxide (0.94/2.03/4)
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2007/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.243(1)
_cell_length_b                   8.243(1)
_cell_length_c                   8.243(1)
_cell_volume                     560.09(12)
_refine_ls_R_factor_all          0.0161
_cod_data_source_file            'data_LiMn2O4melanie155559.cif'
_cod_data_source_block           LiMn2O4melanie155559.cif
_cod_original_cell_volume        560.09
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_database_code               1514030
Crystal growth and structural properties of the spinel-type Li1+x Mn2- x O4 (x = 0.10, 0.14)
Takahashi, Y.; Kijima, N.; Akimoto, J.; Solid State Ionics 177 (2006) 691–695; doi:10.1016/j.ssi.2005.12.025

data_1514031
_publ_section_title
;
 Crystal growth and structural properties of the spinel-type Li1+x Mn2- x
 O4 (x = 0.10, 0.14)
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              691
_journal_page_last               695
_journal_paper_doi               10.1016/j.ssi.2005.12.025
_journal_volume                  177
_journal_year                    2006
_chemical_formula_structural     '(Li1.104 Mn0.896) Mn O4'
_chemical_formula_sum            'Li1.104 Mn1.896 O4'
_chemical_name_systematic
;
Lithium Manganese Oxide (1.1/1.9/4)
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2007/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.2401(9)
_cell_length_b                   8.2401(9)
_cell_length_c                   8.2401(9)
_cell_volume                     559.50(11)
_refine_ls_R_factor_all          0.037
_cod_data_source_file            'data_LiMn2O4melanie155636.cif'
_cod_data_source_block           LiMn2O4melanie155636.cif
_cod_original_cell_volume        559.5
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_database_code               1514031
Crystal growth and structural properties of the spinel-type Li1+x Mn2- x O4 (x = 0.10, 0.14)
Takahashi, Y.; Kijima, N.; Akimoto, J.; Solid State Ionics 177 (2006) 691–695; doi:10.1016/j.ssi.2005.12.025

data_1514032
_publ_section_title
;
 Crystal growth and structural properties of the spinel-type Li1+x Mn2- x
 O4 (x = 0.10, 0.14)
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              691
_journal_page_last               695
_journal_paper_doi               10.1016/j.ssi.2005.12.025
_journal_volume                  177
_journal_year                    2006
_chemical_formula_structural     '(Li1.144 Mn0.856) Mn O4'
_chemical_formula_sum            'Li1.144 Mn1.856 O4'
_chemical_name_systematic
;
Lithium Manganese Oxide (1.14/1.86/4)
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2007/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.2273(10)
_cell_length_b                   8.2273(10)
_cell_length_c                   8.2273(10)
_cell_volume                     556.89(12)
_refine_ls_R_factor_all          0.031
_cod_data_source_file            'data_LiMn2O4melanie155637.cif'
_cod_data_source_block           LiMn2O4melanie155637.cif
_cod_original_cell_volume        556.89
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_database_code               1514032
Structural and electrochemical properties of Li(+) and Co(3+)-codoped Li Mn2 O4
Songtao, Huang; Song, Cao; Su-Rong, Kan; Maoyou, Chu; Shigang, Lu; Jianyun, Shen; Xiyou Jinshu 30 (2006) 129–133; doi:

data_1514033
_publ_section_title
;
 Structural and electrochemical properties of Li(+) and Co(3+)-codoped Li
 Mn2 O4
;
_journal_coden_ASTM              XIJID9
_journal_issue                   2
_journal_name_full               'Xiyou Jinshu'
_journal_page_first              129
_journal_page_last               133
_journal_volume                  30
_journal_year                    2006
_chemical_formula_structural     'Li (Mn2 O4)'
_chemical_formula_sum            'Li Mn2 O4'
_chemical_name_systematic
;
Lithium Manganese(III) Manganese(IV) Oxide
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2007/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.24509(15)
_cell_length_b                   8.24509(15)
_cell_length_c                   8.24509(15)
_cell_volume                     560.514(18)
_refine_ls_R_factor_all          0.0664
_cod_data_source_file            'data_LiMn2O4melanie155665.cif'
_cod_data_source_block           155665-ICSD
_cod_original_cell_volume        560.52
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'Li1 Mn2 O4'
_cod_database_code               1514033
In situ synchrotron diffraction study of high temperature prepared orthorhombic Li Mn O2
Wei, Y.-J.; Ehrenberg, H.; Bramnik, N. N.; Nikolowski, K.; Baehtz, C.; Fuess, H.; Solid State Ionics 178 (2007) 253–257; doi:10.1016/j.ssi.2006.11.018

data_1514034
_publ_section_title
;
 In situ synchrotron diffraction study of high temperature prepared
 orthorhombic Li Mn O2
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              253
_journal_page_last               257
_journal_paper_doi               10.1016/j.ssi.2006.11.018
_journal_volume                  178
_journal_year                    2007
_chemical_formula_structural     'Li (Mn O2)'
_chemical_formula_sum            'Li Mn O2'
_chemical_name_systematic        'Lithium Manganate(III) - Ht'
_space_group_IT_number           59
_symmetry_Int_Tables_number      59
_symmetry_space_group_name_Hall  '-P 2c 2a'
_symmetry_space_group_name_H-M   'P m n m :2'
_audit_creation_date             2007/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            2
_cell_length_a                   4.5725(1)
_cell_length_b                   5.7419(2)
_cell_length_c                   2.8037(1)
_cell_volume                     73.611(4)
_refine_ls_R_factor_all          0.108
_cod_data_source_file            'data_LiMnO2melanie156501.cif'
_cod_data_source_block           LiMnO2melanie156501.cif
_cod_original_cell_volume        73.61
_cod_original_sg_symbol_H-M      'P m n m Z'
_cod_original_formula_sum        'Li1 Mn1 O2'
_cod_database_code               1514034
Characterizations on the structural and electronic properties of thermal lithiated Li0.33 Mn O2
Wei, Y. J.; Ehrenberg, H.; Kim, K. B.; Park, C. W.; Huang, Z. F.; Baehtz, C.; Journal of Alloys and Compounds 470 (2009) 273–277; doi:10.1016/j.jallcom.2008.02.036

data_1514035
_publ_section_title
;
 Characterizations on the structural and electronic properties of thermal
 lithiated Li0.33 Mn O2
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys and Compounds'
_journal_page_first              273
_journal_page_last               277
_journal_paper_doi               10.1016/j.jallcom.2008.02.036
_journal_volume                  470
_journal_year                    2009
_chemical_formula_structural     'Li0.33 (Mn O2)'
_chemical_formula_sum            'Li0.33 Mn O2'
_chemical_name_systematic        'Lithium Manganese Oxide (0.33/1/2)'
_space_group_IT_number           12
_symmetry_Int_Tables_number      12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_audit_creation_date             2009/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 88.3
_cell_angle_gamma                90.
_cell_formula_units_Z            6
_cell_length_a                   13.798(5)
_cell_length_b                   2.839(6)
_cell_length_c                   4.925(2)
_cell_volume                     192.8(4)
_refine_ls_R_factor_all          0.0138
_cod_data_source_file            'data_LiMnO2melanie162591.cif'
_cod_data_source_block           LiMnO2melanie162591.cif
_cod_original_cell_volume        192.84
_cod_original_formula_sum        'Li0.33 Mn1 O2'
_cod_database_code               1514035
X-ray diffraction study on phase transition of orthorhombic Li Mn O2 in electrochemical conversions
Tu, X. Y.; Shu, K. Y.; Journal of Solid State Electrochemistry 12 (2008) 245–249; doi:10.1007/s10008-007-0384-3

data_1514036
_publ_section_title
;
 X-ray diffraction study on phase transition of orthorhombic Li Mn O2 in
 electrochemical conversions
;
_journal_coden_ASTM              JSSEFS
_journal_name_full               'Journal of Solid State Electrochemistry'
_journal_page_first              245
_journal_page_last               249
_journal_paper_doi               10.1007/s10008-007-0384-3
_journal_volume                  12
_journal_year                    2008
_chemical_formula_structural     'Li1.08 Mn1.92 O3.99'
_chemical_formula_sum            'Li1.08 Mn1.92 O3.99'
_chemical_name_systematic
;
Lithium Manganese Oxide (1.08/1.92/4)
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2009/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.241(1)
_cell_length_b                   8.241(1)
_cell_length_c                   8.241(1)
_cell_volume                     559.68(12)
_cod_data_source_file            'data_LiMn2O4melanie163492.cif'
_cod_data_source_block           LiMn2O4melanie163492.cif
_cod_original_cell_volume        559.68
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_database_code               1514036
X-ray diffraction study on phase transition of orthorhombic Li Mn O2 in electrochemical conversions
Tu, X. Y.; Shu, K. Y.; Journal of Solid State Electrochemistry 12 (2008) 245–249; doi:10.1007/s10008-007-0384-3

data_1514037
_publ_section_title
;
 X-ray diffraction study on phase transition of orthorhombic Li Mn O2 in
 electrochemical conversions
;
_journal_coden_ASTM              JSSEFS
_journal_name_full               'Journal of Solid State Electrochemistry'
_journal_page_first              245
_journal_page_last               249
_journal_paper_doi               10.1007/s10008-007-0384-3
_journal_volume                  12
_journal_year                    2008
_chemical_formula_structural     '(Li0.5 Mn0.5) O'
_chemical_formula_sum            'Li0.5 Mn0.5 O'
_chemical_name_systematic        'Lithium Manganese Oxide (0.5/0.5/1)'
_space_group_IT_number           225
_symmetry_Int_Tables_number      225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_audit_creation_date             2009/08/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            4
_cell_length_a                   4.121(3)
_cell_length_b                   4.121(3)
_cell_length_c                   4.121(3)
_cell_volume                     69.99(9)
_cod_data_source_file            'data_LiMnO2melanie163493.cif'
_cod_data_source_block           LiMnO2melanie163493.cif
_cod_original_cell_volume        69.99
_cod_original_formula_sum        'Li0.5 Mn0.5 O1'
_cod_database_code               1514037
Defect spinels in the system (Li2 O) * y(Mn o2) (y>2.5): a neutron- diffraction study and electrochemical characterization of Li2 Mn4 O9
de Kock, A.; Rossouw, M. H.; de Picciotto, L. A.; Thackeray, M. M.; David, W. I. F.; Ibberson, R. M.; Materials Research Bulletin 25 (1990) 657–664; doi:10.1016/0025-5408(90)90032-W

data_1514038
_publ_section_title
;
 Defect spinels in the system (Li2 O) * y(Mn o2) (y>2.5): a neutron-
 diffraction study and electrochemical characterization of Li2 Mn4 O9
;
_journal_coden_ASTM              MRBUAC
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              657
_journal_page_last               664
_journal_paper_doi               10.1016/0025-5408(90)90032-W
_journal_volume                  25
_journal_year                    1990
_chemical_formula_structural     'Li0.83 (Mn1.76 O4)'
_chemical_formula_sum            'Li0.83 Mn1.76 O4'
_chemical_name_systematic
;
Lithium Manganese Oxide (0.83/1.76/4)
;
_space_group_IT_number           227
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2010/02/01
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.174(1)
_cell_length_b                   8.174(1)
_cell_length_c                   8.174(1)
_cell_volume                     546.14(12)
_refine_ls_R_factor_all          0.0153
_cod_data_source_file            'data_LiMn2O4melanie164988.cif'
_cod_data_source_block           LiMn2O4melanie164988.cif
_cod_original_cell_volume        546.14
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_database_code               1514038
_cod_duplicate_entry 1513960